# Abbe number

Jump to: navigation, search

In optics and lens design, the Abbe number, also known as the V-number or constringence of a transparent material, is a measure of the material's dispersion (variation of refractive index versus wavelength), with high values of V indicating low dispersion. It is named after Ernst Abbe (1840–1905), the German physicist who defined it.

Refractive index variation for SF-11 flint glass (upper graph), BK-7 borosilicate glass (middle curve), and fused quartz (dashed curve).

The Abbe number,[1][2] VD, of a material is defined as

$V_D = \frac{ n_D - 1 }{ n_F - n_C },$

where nD, nF and nC are the refractive indices of the material at the wavelengths of the Fraunhofer D-, F- and C- spectral lines (589.3 nm, 486.1 nm and 656.3 nm respectively).

Abbe numbers are used to classify glass and other optical materials in terms of their chromaticity. For example, the higher dispersion flint glasses have V < 55 whereas the lower dispersion crown glasses have larger Abbe numbers. Values of V range from below 25 for very dense flint glasses, around 34 for polycarbonate plastics, up to 65 for common crown glasses, and 75 to 85 for some fluorite and phosphate crown glasses.

Most of the human eye's wavelength sensitivity curve, shown here, is bracketted by the Abbe number reference wavelengths of 486.1 nm (blue) and 656.3 nm (red)

Abbe numbers are used in the design of achromatic lenses, as their reciprocal is proportional to dispersion (slope of refractive index versus wavelength) in the wavelength region where the human eye is most sensitive (see graph). For different wavelength regions, or for higher precision in characterizing a system's chromaticity (such as in the design of apochromats), the full dispersion relation (refractive index as a function of wavelength) is used.

File:Abbe-diagram 2.svg
An Abbe diagram plots the Abbe number against refractive index for a range of different glasses (red dots). Glasses are classified using the Schott Glass letter-number code to reflect their composition and position on the diagram.
Influences of selected glass component additions on the Abbe number of a specific base glass.[3]

An Abbe diagram is produced by plotting the Abbe number Vd of a material versus its refractive index nd. Glasses can then be categorised and selected according to their positions on the diagram. This can be a letter-number code, as used in the Schott Glass catalogue, or a 6-digit glass code.

Glasses' Abbe numbers, along with their mean refractive indices, are used in the calculation of the required refractive powers of the elements of achromatic lenses in order to cancel chromatic aberration to first order. Note that these two parameters which enter into the equations for design of achromatic doublets are exactly what is plotted on an Abbe diagram.

Due to the difficulty and inconvenience in producing sodium and hydrogen lines, alternate definitions of the Abbe number are often substituted (ISO 7944).[4] Rather than the standard definition, above, using the refractive index variation between the F and C hydrogen lines, an alternative measure using the subscript "e"

$V_e = \frac{n_e-1}{ n_{F'} - n_{C'}}$

takes the difference between the refractive indices of the blue and red cadmium lines at 480.0 nm and 643.8 nm (with ne referring to the wavelength of the mercury E-line, 546.073 nm). Other definitions can similarly be employed; the following table lists standard wavelengths at which n is commonly determined, including the standard subscripts employed.[5]

λ in nm Fraunhofer's symbol Light source Color
365.01 i Hg UV
404.66 h Hg violet
435.84 g Hg blue
479.99 F' Cd blue
486.13 F H blue
546.07 e Hg green
587.56 d He yellow
589.3 D Na yellow
643.85 C' Cd red
656.27 C H red
706.52 r He red
768.2 A' K IR
852.11 s Cs IR
1013.98 t Hg IR

## References

1. Hovestadt, H. (1902). Jena Glass and Its Scientific and Industrial Applications. London: Macmillan and Co. pp. 1–81.<templatestyles src="Module:Citation/CS1/styles.css"></templatestyles>
2. Bergmann, Ludwig; Clemens Schaefer (1999). Optics of Waves and Particles. Berlin: Walter de Gruyter. pp. 198–201. ISBN 3-11-014318-6.<templatestyles src="Module:Citation/CS1/styles.css"></templatestyles>
3. Abbe number calculation of glasses
4. Meister, Darryl. "Understanding Reference Wavelengths" (PDF). Carl Zeiss Vision. Retrieved 2013-03-13.<templatestyles src="Module:Citation/CS1/styles.css"></templatestyles>
5. L. D. Pye, V. D. Frechette, N. J. Kreidl: "Borate Glasses"; Plenum Press, New York, 1977